  We calculate the \tco{polarization}-controlled Rayleigh scattering response
of twisted bilayer graphene (tBLG) based on the continuum electronic band model
developed by Bistritzer and MacDonald while considering its refinements which
address the effects of structural corrugation, doping-dependent Hartree
interactions and particle-hole asymmetry. The dominant wave vectors for the
Rayleigh scattering process emanate from various regions of the Moir\'e
Brillouin zone (MBZ) in contrast to single-layer graphene (SLG) and AB-stacked
bilayer graphene (AB-BLG), where the dominant contributions always stem from
the vicinity of the $\bm{K}$ point for optical laser energies and below.
Compared to SLG, the integrated Rayleigh intensity is strongly enhanced for
small twist angles (\emph{e.g.}, at a twist angle $ \theta = 1.2^{\circ} $, the
integrated Rayleigh intensity at laser energy $ E_l=2~\si{\electronvolt} $
enhances by a factor of $\sim $ 100 for the case of parallel
\tco{polarization}). While for the case of cross-\tco{polarization}, it
exhibits a markedly complex \tco{behavior} suggestive of strong interference
effects mediated by the optical matrix elements. We find that at small twist
angles, \emph{e.g.}, $ \theta = 1.05^{\circ} $, the corrugation effects
strongly enhances the ratio $ \bm{R}_A = \frac{ \text{integrated Rayleigh
intensity for parallel \tco{polarization}}}{\text{integrated Rayleigh intensity
for cross-\tco{polarization}}} $ by $ \sim $ $ 1300 $ times \emph{viz a viz}
SLG or AB-BLG.

Mesoscale and Nanoscale Physics;Strongly Correlated Electrons